# Numerical modelling of lubricated foil rolling

## Texte intégral

(1)

A model of lubricated cold strip rolling (1, 2) is extended to the thin foil regime. The model considers the evolution of asperity geometry and lubricant pressure through the bite, treating the strip using a conventional slab model. The elastic deflections of the rolls are coupled into the problem using an elastic finite element model.

Friction between the roll and the asperities on the strip is modelled using the Coulomb and Tresca friction factor approaches. The shear stress in the Coulomb friction model is limited to the shear yield stress of the strip. A novel

modification to these standard friction laws is used to mimic slipping friction in the reduction regions and sticking friction in a central neutral zone. The model is able to reproduce the sticking and slipping zones predicted by Fleck et al. (3).

The variation of rolling load, lubricant film thickness and asperity contact area with rolling speed is examined, for conditions typical of rolling aluminium foil from a thickness of 50 to 25µm. The contact area and hence friction rises as the speed drops, leading to a large increase in rolling load. This increase is considerably more marked using Coulomb friction as compared with the friction factor approach. Forward slip

increases markedly as the speed falls and a significant sticking region develops.

INTRODUCTION

Industry is increasingly concerned to develop models of cold rolling, both to improve their on-line control, and to optimize mill set-up and scheduling. Two factors make foil modelling particularly demanding. Firstly, it is essential to model the elastic deformation of the rolls accurately. Secondly, as the ratio of the bite length to the strip thickness increases, the load and reduction in gauge become increasingly sensitive to friction, requiring an accurate mathematical model of friction.

The foil rolling model of Fleck et al (3), which has become widely accepted in industry, combines elastic deformation of the rolls and an elastic-plastic model of the foil. They assume that friction between the roll and strip can be modelled using a Coulomb friction coefficient, typically using a value of 0.03.

The contact length is split into a series of zones, depending on whether the strip is plastic or elastic and whether there is slip between the roll and strip. At the thinner gauges the solution predicts a central flat, no-slip region, where friction falls below the limiting value for slipping. This model has been extended by Dixon and Yuen (4) and Domanti et al (5).

An alternative strategy which overcomes numerical difficul- ties associated with the above procedure is described by Gratacos et al (6). They define an arbitrary friction law which simulates sticking friction in the neutral zone and slipping friction elsewhere. Le and Sutcliffe (7) extend this approach using a physically-based friction law in the neutral zone.

An approximation to the lubrication conditions in the contact can be made by estimating the oil film thickness hs accor- ding to Wilson and Walowit’s (8) formula for smooth rolls and strips :



where u–

= (ur+ us0)/2 is the mean of the roll and strip inlet speeds, θ0is the inlet angle between the strip and roll and Y is the plain strain yield strength of the strip. η0is the visco- sity of the lubricant at ambient pressure and αis the Barus pressure viscosity coefficient. The ratio Λs = hst0 of the smooth film thickness hsto the combined roll and initial strip roughness σt0is used to characterize the lubrication regime.

In industrial rolling, the needs for high productivity but good surface finish dictate that rolling is commonly in the “mixed”

regime with Λsbetween 0.01 and 0.5.

## Numerical modelling of lubricated foil rolling

### M.P.F. Sutcliffe*, P. Montmitonnet**

* Department of Engineering,

University of Cambridge, Grande-Bretagne

** CEMEF, École des Mines de Paris, Sophia Antipolis

Manuscrit reçu le 20 juin 2000, bon à publier le 5 octobre 2000.

© La Revue de Métallurgie 2001.

(2)

Various tribological models have been described recently for cold strip rolling (2, 9-12). The change in oil pressure is modelled using Reynolds equation, suitably modified to include the effect of roughness. The effect of bulk deforma- tion on the asperity crushing behaviour can be described using the results of Sutcliffe (13) or Wilson and Sheu (14).

Two approaches have been used to combine the lubrication details with an overall model of the bite. Either an inlet ana- lysis can be used, in which it is assumed that the tribology of the contact is determined in a short inlet region (11).

Alternatively, the plasticity and tribological details are model- led through the bite (9, 10, 12). These models calculate the variation of lubricant film thickness through the bite and hence the area of contact ratio A, i.e. the fraction of the sur- face for which the asperity tops are in contact. The remai-

ning valley regions are separated by oil. The friction stress is found by adding contributions from these two areas.

Results show that the film thickness and area of contact ratio depend primarily on the rolling speed, oil properties and inlet geometry. The effects of yield stress, strip thickness, asperity geometry and unwind tension are of secondary importance.

Experimental measurements of film thickness are in good agreement with theoretical predictions (10, 15).

For foil rolling, it is necessary to model both roll elastic defor- mation and the tribology. Marsault et al. (1, 2) describe such a model, but only consider the case where there is limited roll elasticity. In this paper that model is extended to the thin foil regime where there is a central flat section.

Le laminage des métaux en feuille mince met en œuvre un fort couplage entre la déformation des cylindres et celle de la feuille, qui se traduit par de sérieuses diffi- cultés de convergence des modèles d’une part, et une mécanique particulière : très grande sensibilité au frot- tement (donc à la lubrification), contact des cylindres de part et d’autre de la feuille (« roll kiss »), apparition d’une zone très déformée, quasi-plate, sur la surface de contact avec le cylindre, où le métal, en déformation élastique, a la vitesse du cylindre (« zone collante » ou

« zone neutre »).

Le modèle de lubrification en régime mixte du laminage à froid de tôle (1, 2) présenté dans ce numéro (Montmitonnet et al.) a donc été adapté à ce laminage en très faible épaisseur. Il prend en compte l’évolution de la géométrie des aspérités et de la pression du lubri- fiant le long de l’emprise , la tôle étant traitée par un modèle de tranches classique [5[, . On y couple la déformation élastique des cylindres, dont le calcul fait appel à la méthode des éléments finis. Le frottement entre le cylindre et la rugosité de la tôle est représenté au choix par les modèles de Coulomb ou de Tresca .

Dans le premier cas, la contrainte de cisaillement est limitée par la contrainte d’écoulement en cisaillement de la tôle. On introduit une nouvelle modification à ces lois standard (équ. , fig. 1) pour simuler le frottement glis- sant dans les zones de réduction et le frottement collant dans la zone neutre centrale. Le modèle est ainsi capable de reproduire la co-existence de zones glissantes et collantes (fig. 2 et 4) prédites par Fleck et al. (3).

On examine les variations de force de laminage, d’épaisseur de film lubrifiant et d’aire réelle de contact avec la vitesse de laminage, pour des conditions typiques du laminage d’aluminium en feuille mince, de 50 à 25µm. L’aire réelle de contact, donc le frottement, croît lorsque la vitesse diminue, du fait du moindre entraînement d’huile par effet hydrodynamique. Cela provoque une augmentation de la force de laminage (jusqu’à un facteur 40 entre 40 m.s-1 et 10 m.s-1 !), considérablement plus marquée si on utilise un frotte- ment de Coulomb plutôt que celui de Tresca. Le glisse- ment en avant augmente notablement quand la vitesse diminue, atteignant les très hautes valeurs rencontrées en pratique (jusqu’à 45 %, pour une réduction d’épais- seur de 50 %). La réduction s’effectue exclusivement en entrée et sortie de l’emprise (voir fig. 3), l’épaisseur de la feuille restant constante dans la partie centrale, où le contact est d’ailleurs collant (vitesse relative nulle).

On compare la loi de Coulomb et la loi de Tresca, les valeurs des coefficients (µa= 0,1, ma= 0,25) étant choi- sies pour donner la même force de laminage à grande vitesse. La loi de Tresca se caractérise par l’absence d’effet « boule-de-neige » que subit la loi de Coulomb (lorsque la vitesse diminue, le frottement augmente ; la pression de contact croît rapidement, ce qui augmente les contraintes de frottement, et ainsi de suite). Les variations de la force ou du glissement en avant avec la vitesse sont donc ralenties.

### M.P.F. Sutcliffe*, P. Montmitonnet**

* Department of Engineering,

University of Cambridge, Grande-Bretagne

** CEMEF, École des Mines de Paris, Sophia Antipolis

(3)

THEORY

Most of the modelling and numerical implementation is taken directly from the work of Marsault (1) and only an out- line is given here. To extend the model into the thin foil regime where the roll deformations are large, a new friction model is introduced, as described below, to overcome numerical difficulties with Marsault’s formulation.

### Friction modelling

Fleck et al (3) show that both slipping and sticking between the roll and strip need to be considered in foil rolling. For the regions of slipping, either a Coulomb friction coefficient µaor a Tresca friction factor ma is used to estimate the shear stress τaon the asperity tops as :



where pa is the pressure on the asperity tops and k is the shear yield stress of the workpiece. With the Coulomb fric- tion model, it is necessary to include the additional limitation that the friction stress cannot exceed the shear yield stress of the strip. With the slab model used to model the strip, fric- tional shear stresses are not included when considering the yield condition for the strip, so that this limit is not otherwise imposed.

To simulate the sticking region, where the shear stress falls below the value for slipping friction (equation ), the approach of Gratacos et al (6) is followed in adopting an arbitrary friction law. A knockdown factor δon the limiting friction is applied to , so that τa= δµapaor δmak, with :



where ε is a tolerance parameter, θ the local roll slope and θ1a representative roll slope in a slipping region (see fig. 3). Here θ1is taken as the slope at the middle of the first reduction region. This variation of δwith θ/θ1is sketched in figure 1. For θ/θ1 «ε the frictional stress is approximately proportional to the roll slope while, for θ/θ1» ε, δapproaches one and friction takes its limiting value of µapa or mak.

Changes in friction in the central sticking region can be accommodated by small deviations in flatness. As long as ε is sufficiently small, the roll stays essentially flat there and the solution is unaffected by the exact form of the friction law.

Typically a value of ε= 0.1 was found appropriate. A physi- cally-based argument for a friction law of this form is pre- sented by Le and Sutcliffe (7).

The shear stress in the valleys τb is estimated from the Newtonian viscous behaviour of the oil, with a constant val- ley depth of ht/(1-A), where htis the mean film thickness. The lesser of this hydrodynamic estimate and the corresponding shear stress τa on the asperity tops is used for the valley regions. The average shear stress τis given by a weighted sum of the asperity and valley contributions :



### laminage de films minces

NOTATIONS

A : area of contact ratio

ht : mean film thickness, averaged across the width of the contact

hs : smooth film thickness, using the Wilson and Walowit formula, equation 

k : shear yield stress of the strip (k = Y/√ 3for the von Mises yield criterion).

ma, mb : friction factor for the areas of contact and valleys p : mean contact pressure between roll and strip pa, pb : pressure on the asperity tops and in the valleys R : roll radius

t, t0: strip thickness, inlet thickness u– : mean entraining velocity, u= (ur+ us)/2 ur, us(us0): roll and strip speed (at the inlet) x : co-ordinate in rolling direction Y : plane strain yield stress of the strip α : oil pressure viscosity index

δ : Knock-down factor for frictional stress in the sticking region

ε : tolerance for strip slope in sticking region η (η0): viscosity of lubricant (at ambient pressure) λ : wavelength of the surface roughness Λs : speed parameter,Λs= hs/σt0

µa, µb: Coulomb friction coefficient for the areas of contact and valleys

θ, θ0, θ1: roll slope, at the inlet and at a representative point in the bite (see fig. 3)

σt, (σt0): combined r.m.s. surface roughness of the strip and roll (initial roughness)

σx : longitudinal tension stress

τ : mean shear stress between roll and strip τa, τb: shear stress for the areas of contact and valleys

Figure 1 – Schematic variation in knockdown factor δwith roll slope θused to simulate sticking and slipping friction.

Figure 1 – Schéma des variations du facteur d’atténuation δ en fonction de la pente θde la surface du cylindre, tel qu’utilisé

pour simuler le frottement glissant et le frottement collant.

(4)

### Strip deformation

A standard slab model is used for the strip. Equilibrium for a slab in the bite gives :



where x is the distance in the rolling direction, t the strip thickness, σxthe tensile stress in the rolling direction and p the average contact pressure. In the inlet and exit regions, where there is no plastic deformation, it is assumed that the strip is linear-elastic. In the central reduction region, the strip is taken as perfectly plastic, and at the point of yield, so that :

σx+ p = Y 

In principle there can be elastic unloading in the flat central region of the bite. However, as long as the roll remains essentially flat in this region, this detail can be neglected. In these circumstances, the pressure distribution is effectively independent of the constitutive model in this region, instead being determined by the pressure needed to generate a flat on the roll.

### Roll elasticity

A standard elastic FEM package is used to solve the roll deformation equations for a given pressure distribution. The roll surface deformations relative to the centre of the roll are calculated and the approach of centres of the rolls updated between iterations to maintain a constant strip reduction.

Cubic splines are used to interpolate between node points in the FE model for integrating the hydrodynamic equations.

### Hydrodynamic modelling

The variation in oil pressure pb through the bite is given by Reynolds equation, modified to include the effect of roughness :



where uxis the local strip velocity and Qa flow rate constant.

Flow factors φxand φs, which are functions of the mean film thickness htand the combined strip and roll roughness σt, are derived by Wilson and Marsault (16), using the results of Patir and Cheng (17) and Lo (18). They also depend on γ, the ratio of roughness correlation lengths in the rolling and transverse direction. Here γis taken equal to 9, appropriate for nearly longitudinal roughness. To avoid numerical insta- bilities, the Poiseuille term is dropped in the work zone where appropriate. As the oil film becomes smaller, Lo shows that a ‘percolation threshold’ is eventually reached when individual pockets of oil become trapped. This occurs, for longitudinal roughness with γ= 9, when ht/σt= 0,038. For the results presented here, the film thicknesses are signifi- cantly greater than this percolation threshold. Where the film thickness approaches the percolation threshold, micro- plasto-hydrodynamic models are needed (19).

### Asperity Flattening

To derive an accurate estimate of the change in asperity geometry and contact area through the bite, it is essential to include the effect of bulk plasticity on changes in asperity deformation. Here Sutcliffe’s (20) model for crushing of longitudinal roughness is used. This uses a curve fit to the finite element calculations of Korzekwa (21), and is qualita- tively similar to the asperity crushing model of Sheu and Wilson (14).

### Numerical method

The details of the numerical method are described in detail by Marsault et al. (1, 2). A double-shooting procedure is used to find the inlet strip speed and oil flow rate constant Q for a given roll shape. The differential equations for the variation of pressure and contact ratio through the bite are integrated using a Runge-Kutta method. As the integration proceeds, the appropriate equations are changed, according to the local conditions (e.g. elastic or plastic strip, inclusion of the Poiseuille term in the Reynolds equation). Once a converged pressure distribution is found, the corresponding strip shape tC is solved using the FE model for the roll elastic deformations. The roll shape is updated using a relaxation method, until the change in roll shape is within a suitably small tolerance. The new roll shapetN+1is related to the old roll shape tN and the computed roll shape tC, based on the current pressure distribution, by the relaxation formula :



Typically a relaxation coefficient βbetween 0.2 and 0.05 is suitable, giving computation times of the order of 2 h on a small super-computer for the most demanding cases.

RESULTS

In this section we present results typical of industrial rolling of aluminium foil from a thickness of 50 to 25µm, lubricated with a standard rolling oil. For these conditions there is significant roll elasticity. Coiling tensions are applied on the unwind and rewind sides. Conditions are detailed in table I.

Figure 2 shows the distribution of average pressure p, ave- rage shear stress τand area of contact ratio Afor a rolling speed of 20 m/s with a Coulomb friction factor µa= 0.1. The normal pressure is normalized by the yield stress Yand the shear stress by µaY, so that the shear curve lies on the pres- sure curve when the effective contact area Aand the friction knockdown factor δare both equal to one. Figure 3 shows the corresponding change in strip thickness t through the bite, normalised by the inlet strip thicknesst0. These results have a similar form to those of Fleck et al. (3), with a signifi- cant « flat » sticking region at the centre of the bite where the shear stress fall below its limiting value. Because of the friction law used, there are in fact small deviations in thick- ness in this central region, but these are so slight as to be

(5)

scarcely visible in figure 3. The relaxation technique used to update the roll shape has converged automatically on the shape in the central flat region which gives the appropriate sticking friction distribution compatible with the elastic defor- mations of the roll. Figure 2 shows that, for the Coulomb friction model, the frictional stress equals the shear yield stress of the strip over a significant portion of the exit reduc- tion region (where the shear stress has a plateau). Because of the high pressures directly after this region of the bite, the estimated hydrodynamic shear stress would exceed the asperity shear stress. Hence the average shear stress is taken equal to µap, the effective contact area equals one and the curves for shear and normal pressure lie on top of one another.

Details at the inlet are illustrated in figure 4, showing the change in normal pressure p, asperity and hydrodynamic pressures paand pband area of contact ratio A. Comparing the scales on figures 2 and 4 it is clear that the inlet region is very short compared with the length of the bite. At the beginning of the inlet, before the hydrodynamic pressure has built up, the asperity pressure is approximately equal to the hardness 3Y. As the pressure in the lubricant build ups, the strip yields, causing a sharp change in the slope of the mean pressure curve and a drop in the asperity pressure.

At this point, the asperity tops are rapidly flattened and the valley pressure rapidly rises to equal the asperity pressure.

### laminage de films minces

Figure 3 – Variation in strip thickness through the bite, ur= 20 m/s, µa= 0.1. Angle θis the local slope of the roll profile, θ0its value at bite entry, θ1at the centre of the first

deformation zone.

Figure 3 – Variation le long de l’emprise de l’épaisseur de la tôle. ur= 20 m/s, µa= 0,1. L’angle θest la pente locale au profil du cylindre, θ0sa valeur au point d’entrée, θ1au centre

de la première zone de déformation.

TABLE I – Summary of conditions.

TABLEAU I – Résumé des conditions de laminage.

Strip Entry gauge Exit gauge Yield stress Unwind tension Rewind tension Young's modulus Poisson's ratio

50 µm 25 µm 150 MPa

20 MPa 20 MPa 70 Gpa

0.3

Roll peripheral speed Young's modulus Poisson's ratio

135 mm 5 - 40 m/s

210 GPa 0.3 Surfaces Combined r.m.s. amplitude

Asperity wavelength Asperity friction

0.3 µm 30 µm µa = 0.1 orma = 0.25 Lubricant Viscosity at ambient pressure

Pressure viscosity coefficient

2.5× 10-3 Pas 1.2× 10-8 m2/N

Figure 2 – Variation in pressure, shear stress and area of contact ratio through the bite ; ur= 20 m/s, µa= 0.1.

Figure 2 – Variation le long de l’emprise de la pression de contact, de la contrainte de cisaillement et de l’aire réelle de contact ;

ur= 20 m/s, µa= 0,1.

Figure 4 – Variation of asperity, valley and average pressure and area of contact ratio in the inlet ; ur= 20 m/s, µa= 0.1.

Figure 4 – Zone d’entrée : variation des pressions sur les aspérités, dans les vallées et moyenne, ainsi que de l’aire réelle

de contact ; ur= 20 m/s, µa= 0,1.

(6)

Through the remainder of the bite, the model assumes that the valley pressure pbremains equal to the asperity pressure pa. The area of contact ratio Aincreases slightly through the rest of the bite due to thinning of the oil film as the strip sur- face elongates,fig. 2.

Figure 5 shows the variation through the bite of the normal pressure p, the shear stress τand area of contact ratio A, for the same conditions as figure 2, but with a friction factor ma = 0.25 instead of a friction coefficient µa = 0.1. These values of friction factor and friction coefficient have been chosen for comparison to give approximately the same mean frictional stress and rolling loads at high rolling speeds where there is only a slight friction hill. (In fact the two laws give the same stress for p= 1.4Y.) The friction factor approach gives lower shear stresses in the high pressure regions where p> 1.4Y, and so a significantly lower average pressure. The frictional stresses are normalised by maY/√–

3, so that this expression equals one when the effective contact area and the friction knockdown factor δare both equal to one.

### Effect of speed

Figure 6 shows the effect of rolling speed on roll load, using a logarithmic axis for load. The change in speed from 5 to 40 m/s corresponds to a range of film thickness parameter Λsfrom 0.22 to 1.76(*). The graph includes the cases of a friction coefficient of 0.1 and a Tresca friction factor of 0.25.

Corresponding changes in the forward slip and the mean film thickness ht/σt0and area of contact ratio Aat the exit are plotted in figure 7. As the speed falls, there is a reduction in the thickness of the oil film drawn through the contact ht/σt0

and the area of contact ratio rises accordingly. The associa- ted increase in frictional stress causes a large increase in rolling load, as observed experimentally. A flat region in the bite is predicted below speeds of about 20 and 30 m/s for

the friction coefficient and friction factor approaches, res- pectively. The marked difference in load between the Tresca and Coulomb friction models, fig. 6, reflects the sensitivity of results to the details of the friction distribution, despite the relatively slight changes in the film thickness and area of contact estimates (fig. 7).

Forward slip is a useful indicator of the strip shape in the bite, as well as being an important variable for control pur- poses. Figure 7 shows that an increase in forward slip from about 5 to 45 % is predicted with the Coulomb model as the speed falls and a flat central region develops. The increase in forward slip is much less marked for the Tresca friction model. There are larger frictional tractions at the exit than at the entry, both on account of the increase in area of contact ratio through the bite and due to the larger hydrodynamic friction component at the higher pressures in the exit half of the bite. This tends to inhibit strip reduction at the exit leading to smaller values of forward slip than predicted by the constant friction coefficient model of Fleck et al (3).

Figure 5 – Variation in pressure, shear stress, and area of contact ratio through the bite ; ur= 20 m/s, ma= 0.25.

Figure 5 – Variation le long de l’emprise de la pression de contact, de la contrainte de cisaillement et de l’aire réelle de contact ;

ur= 20 m/s, ma= 0,25.

Figure 6 – Effect of rolling speed on roll load.

Figure 6 – Effet de la vitesse sur la force de laminage.

Figure 7 – Effect of rolling speed on area of contact ratio, film thickness and forward slip.

Figure 7 – Effet de la vitesse sur l’aire réelle de contact, l’épaisseur de film et le glissement en avant.

* Although the smooth film thickness, equation , is based on the slope of the undeformed roll at the inlet, in fact the slope of the deformed roll is not very different for the cases presented here. Hence this smooth film thickness is representative.

(7)

DISCUSSION

Figures 6 and 7 confirm that the key rolling parameters – load and forward slip – are sensitive to the details of the fric- tional model. An appropriate choice of friction model must rely either on a comparison with experimental measure- ments or some physical insight into the interface behaviour in the bite. Both approaches are currently being explored. As figure 4 shows, the inlet region is very short compared with the bite region for the conditions considered here. Sutcliffe and Johnson (11) explained why this could be expected with mixed lubrication and typical roll roughnesses and strip reductions, while Le and Sutcliffe (22) have constructed a regime map for thick strip rolling which shows that this is true for most practical purposes. With foil rolling, the small value of t/λ, the ratio of the strip thickness to the roughness wave- length, increases the ease with which asperities can be cru- shed. Hence the inlet will be small compared with the bite over an even wider range of operating conditions. This observation suggests that it would be appropriate in most cases to consider all the tribological details only in the inlet.

A much-simplified model of the contact could be used to estimate the change in friction through the bite. With this approach there is limited coupling between roll deformation and lubrication, which would give a much simpler and more robust analysis.

The characteristic roughness wavelength λwas taken in this analysis as 30µm. Sutcliffe and Le (20, 22) investigate the effect of roughness wavelength, considering more than one wavelength. Their results and subsequent work in progress suggest this single value characterizes the spectrum of roughness reasonably well for typical aluminium foil rolling conditions.

CONCLUSIONS

A tribological model of cold strip rolling (1, 2) is extended to the thin foil rolling where the elastic deflections of the rolls become significant. This model calculates the variation of asperity geometry and lubricant pressure through the bite and uses a conventional slab model of the strip. An elastic finite element model is used to calculate roll deflections. A previous model of foil rolling (3) predicts reduction zones at the entry and exit to the bite, with a flat neutral zone where there is limited relative slip between the roll and strip. This observation is used to construct an arbitrary modification to the standard friction laws which simulates this behaviour, with friction proportional to the roll slope in the sticking region and equal to the limiting friction value in the slipping regions. Either Coulomb and Tresca friction models are used in the slipping regions for contact between the rolls and asperity tops, while the frictional stress in the valleys is esti- mated from the viscous shearing of the oil. In the case of Coulomb friction, the frictional stress is limited to the shear yield stress of the strip.

Results are calculated for typical industrial conditions, rolling aluminium foil from a thickness of 50 to 25µm. In a short inlet region, the pressure rises in the lubricant until bulk yiel-

ding takes place. At that point the asperities are rapidly cru- shed until the lubricant and asperity pressures equalize.

Through the rest of the bite there is a more modest increase in area of contact ratio associated with thinning of the oil film as the strip elongates. Predictions of rolling load using Coulomb friction are significantly higher than those using a friction factor approach. A correct choice of friction model will depend on experimental observations or further physical insight into the behaviour in the bite. The effect of a variation in rolling speed from 5 to 40 m/s on rolling load, film thick- ness and contact area is examined. As the speed falls, there is a decrease in the amount of oil drawn into the bite and so an increase in area of contact ratio. The associated increase in friction causes a significant increase in rolling load. This is in line with experimental observations. As the speed falls, the forward slip is predicted to increase from a value of 5 to 45 % for the Coulomb friction model. The increase in for- ward slip is much less marked for the Tresca friction model.

Finally, it is suggested that in many circumstances it would be appropriate to simplify the model by calculating the details of the tribology only in the short inlet region. This would improve convergence and robustness considerably.

### Acknowledgements

The authors are most grateful for the advice provided by Drs. Gratacos and Marsault and for the financial help and equipment provided by the CEMEF group at the École des Mines de Paris.

## references

(1) MARSAULT (N.) – Modélisation du régime de lubrification mixte en laminage à froid. PhD Thesis, École Nationale Supérieure des Mines de Paris (1998).

(2) MARSAULT (N.), MONTMITONNET (P.), DENEUVILLE (P.), GRATACOS (P.) – A model of mixed lubrication for cold rolling of strip. Proc. NUMIFORM 98, Twente University, Netherlands, A.A. Balkema (Rotterdam) (1998), p. 715-720.

(3) FLECK (N.A.), JOHNSON (K.L.), MEAR (M.E.), ZHANG (L.C.) – Cold rolling of foil. Proc. Instn. Mech. Engrs, 206 (1992), p. 119-131.

(4) DIXON (A.E.), YUEN (W.Y.D.) – A computationally fast method to model thin strip rolling. Proc. Computational Techniques and Application Conference (1995), p. 239-246.

(5) DOMANTI (S.A.), EDWARDS (W.J.), THOMAS (P.J.), CHEF- NEUX (L.) – Application of foil rolling models to thin steel strip and temper rolling. Proc. 6th International Rolling Conference, Düsseldorf (1994), p. 422-429.

(6) GRATACOS (P.), MONTMITONNET (P.), FROMHOLZ (C.), CHENOT (J.L.) – A plane-strain elastic finite-element model for cold rolling of thin strip. Int. J. Mech. Sci., 34, 3 (1992), p. 195-210.

(7) LE (H.R.), SUTCLIFFE (M.P.F.) – A robust model for rolling of thin strip and foil. Int. J. Mech. Sci, 43 (1999), 1405-1419.

(8) WILSON (W.R.D.), WALOWIT (J.A.) – An isothermal hydro- dynamic lubrication theory for strip rolling with front and back tension. Proc. 1971 Tribology Convention, I. Mech. E., London (1972), p. 164-172.

### laminage de films minces

(8)

(9) LIN (H.S.), MARSAULT (N.), WILSON (W.R.D.) – A mixed lubrication model for cold strip rolling. Part I. Theoretical.

Tribology Trans., 41 (1998), p. 317-326.

(10) SHEU (S.), WILSON (W.R.D.) – Mixed lubrication of strip rol- ling. STLE Trib. Trans., 37 (1994), p. 483-493.

(11) SUTCLIFFE (M.P.F.), JOHNSON (K.L.) – Lubrication in cold strip rolling in the “mixed” regime. Proc. Instn. Mech. Engrs., 204 (1990), p. 249-261.

(12) CHANG (D.F.), WILSON (W.R.D.), MARSAULT (N.) – Lubrication of strip rolling in the low-speed mixed regime.

Trib. Trans., 39 (1996), p. 407-415.

(13) SUTCLIFFE (M.P.F.) – Surface asperity deformation in metal forming processes. Int. J. of Mech. Sci., 30 (1988), p. 847- 868.

(14) WILSON (W.R.D.), SHEU (S.) – Real area of contact and boundary friction in metal forming. Int. J. Mech. Sci., 30 (1988), p. 475-489.

(15) SUTCLIFFE (M.P.F.), JOHNSON (K.L.) – Experimental mea- surements of lubricant film thickness in cold strip rolling.

Proc. Instn Mech. Engrs., 204 (1990), p. 263-273.

(16) WILSON (W.R.D.), MARSAULT (N.) – Partial hydrodynamic lubrication with large fractional contact areas. ASME J. Tribology, 120 (1998), p. 1-5.

(17) PATIR (N.), CHENG (H.S.) – An average flow model for deter- mining effects of three dimensional roughness on partial hydrodynamic lubrication. ASME J. Lubrication Techno- logy, 100 (1978), p. 12-17.

(18) LO (S.W.) – A study on the flow phenomena in the mixed lubrication regime by porous medium model. ASME J.

Tribology, 116 (1994), p. 640-647.

(19) LO (S.W.), WILSON (W.R.D.) – A theoretical model of micro- pool lubrication in metal forming, ASME J. of Tribology, 121 (1999), p. 731-738.

(20) SUTCLIFFE (M.P.F.) – Flattening of random rough surfaces in metal forming processes. ASME J. Tribology, 121 (1999), p. 433-440.

(21) KORZEKWA (D.A.) – Surface asperity deformation during sheet forming. Int. J. Mech. Sci., 34, 7 (1992), p. 521-539.

(22) SUTCLIFFE (M.P.F.), LE (H.R.) – Measurements of surface roughness in cold metal rolling in mixed lubrication regime.

STLE Trib. Trans., 43 (2000), p. 39-44.

Updating...

## Références

Updating...

Sujets connexes :